#------------------------------------------------------------------------------
#$Date: 2019-11-25 19:26:53 +0200 (Mon, 25 Nov 2019) $
#$Revision: 241635 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/13/14/4131435.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4131435
loop_
_publ_author_name
'Haynes, Alyssa S.'
'Stoumpos, Constantinos C.'
'Chen, Haijie'
'Chica, Daniel'
'Kanatzidis, Mercouri G.'
_publ_section_title
;
 Panoramic Synthesis as an Effective Materials Discovery Tool: The System
 Cs/Sn/P/Se as a Test Case.
;
_journal_issue                   31
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              10814
_journal_page_last               10821
_journal_paper_doi               10.1021/jacs.7b05423
_journal_volume                  139
_journal_year                    2017
_chemical_formula_moiety         Cs4SnP4Se12
_chemical_formula_sum            'Cs4 P4 Se12 Sn'
_chemical_formula_weight         1721.73
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_H-M   'R -3 :H'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   7.8083(11)
_cell_length_b                   7.8083(11)
_cell_length_c                   37.905(8)
_cell_measurement_reflns_used    5141
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.73
_cell_measurement_theta_min      1.61
_cell_volume                     2001.4(6)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 6.67
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_measurement_method       rotation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0769
_diffrn_reflns_av_sigmaI/netI    0.0435
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       47
_diffrn_reflns_limit_l_min       -47
_diffrn_reflns_number            5141
_diffrn_reflns_theta_full        26.73
_diffrn_reflns_theta_max         26.73
_diffrn_reflns_theta_min         1.61
_exptl_absorpt_coefficient_mu    22.932
_exptl_absorpt_correction_T_max  0.7356
_exptl_absorpt_correction_T_min  0.3512
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'STOE X-RED32'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.285
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             2214
_exptl_crystal_size_max          0.062
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.015
_refine_diff_density_max         1.505
_refine_diff_density_min         -1.172
_refine_diff_density_rms         0.183
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.054
_refine_ls_matrix_type           full
_refine_ls_number_parameters     63
_refine_ls_number_reflns         942
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.053
_refine_ls_R_factor_all          0.0930
_refine_ls_R_factor_gt           0.0566
_refine_ls_shift/su_max          0.029
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0349P)²+50.7370P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1085
_refine_ls_wR_factor_ref         0.1241
_reflns_number_gt                638
_reflns_number_total             942
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja7b05423_si_002.cif
_cod_data_source_block           Cs4SnP4Se12
_cod_original_sg_symbol_H-M      R-3
_cod_database_code               4131435
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sn1 Sn 1.0000 1.0000 0.5000 0.0486(6) Uani 1 6 d S
Cs2 Cs 0.3333 0.6667 0.36894(3) 0.0763(5) Uani 1 3 d S
Cs3 Cs 0.6667 0.3333 0.45495(4) 0.1013(7) Uani 1 3 d S
Se4 Se 0.6915(12) 0.845(5) 0.45811(17) 0.0474(14) Uani 0.401(4) 1 d P
Se4A Se 0.677(2) 0.886(2) 0.4564(4) 0.0474(14) Uani 0.30(3) 1 d P
Se4B Se 0.680(2) 0.793(3) 0.4565(4) 0.0474(14) Uani 0.30(3) 1 d P
Se5 Se 0.834(3) 0.6595(10) 0.37611(18) 0.0633(15) Uani 0.747(4) 1 d P
Se5A Se 0.793(7) 0.671(4) 0.3797(7) 0.0633(15) Uani 0.18(3) 1 d P
Se5B Se 0.900(13) 0.682(7) 0.3804(13) 0.0633(15) Uani 0.07(3) 1 d P
P06 P 0.8520(13) 0.9264(14) 0.40510(19) 0.044(2) Uani 0.33 1 d P
P07 P 0.9138(14) 0.8278(13) 0.4197(2) 0.045(2) Uani 0.33 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Se4 Sn1 Se4 179.998(7) . 10_776
Se4 Sn1 Se4 92.89(19) . 11_566
Se4 Sn1 Se4 87.11(19) 10_776 11_566
Se4 Sn1 Se4 87.11(19) . 2_765
Se4 Sn1 Se4 92.89(19) 10_776 2_765
Se4 Sn1 Se4 180.0(2) 11_566 2_765
Se4 Sn1 Se4 92.9(2) . 12_656
Se4 Sn1 Se4 87.11(19) 10_776 12_656
Se4 Sn1 Se4 87.11(19) 11_566 12_656
Se4 Sn1 Se4 92.89(19) 2_765 12_656
Se4 Sn1 Se4 87.11(19) . 3_675
Se4 Sn1 Se4 92.9(2) 10_776 3_675
Se4 Sn1 Se4 92.89(19) 11_566 3_675
Se4 Sn1 Se4 87.11(19) 2_765 3_675
Se4 Sn1 Se4 180.000(10) 12_656 3_675
Se4 Sn1 Se4B 7.6(6) . .
Se4 Sn1 Se4B 172.4(6) 10_776 .
Se4 Sn1 Se4B 98.1(5) 11_566 .
Se4 Sn1 Se4B 81.9(5) 2_765 .
Se4 Sn1 Se4B 87.6(4) 12_656 .
Se4 Sn1 Se4B 92.4(4) 3_675 .
Se4 Sn1 Se4B 172.4(6) . 10_776
Se4 Sn1 Se4B 7.6(6) 10_776 10_776
Se4 Sn1 Se4B 81.9(5) 11_566 10_776
Se4 Sn1 Se4B 98.1(5) 2_765 10_776
Se4 Sn1 Se4B 92.4(4) 12_656 10_776
Se4 Sn1 Se4B 87.6(4) 3_675 10_776
Se4B Sn1 Se4B 180.0(5) . 10_776
Se4 Sn1 Se4B 87.6(4) . 11_566
Se4 Sn1 Se4B 92.4(4) 10_776 11_566
Se4 Sn1 Se4B 7.6(6) 11_566 11_566
Se4 Sn1 Se4B 172.4(6) 2_765 11_566
Se4 Sn1 Se4B 81.9(5) 12_656 11_566
Se4 Sn1 Se4B 98.1(5) 3_675 11_566
Se4B Sn1 Se4B 92.3(4) . 11_566
Se4B Sn1 Se4B 87.7(4) 10_776 11_566
Se4 Sn1 Se4B 92.4(4) . 2_765
Se4 Sn1 Se4B 87.6(4) 10_776 2_765
Se4 Sn1 Se4B 172.4(6) 11_566 2_765
Se4 Sn1 Se4B 7.6(6) 2_765 2_765
Se4 Sn1 Se4B 98.1(5) 12_656 2_765
Se4 Sn1 Se4B 81.9(5) 3_675 2_765
Se4B Sn1 Se4B 87.7(4) . 2_765
Se4B Sn1 Se4B 92.3(4) 10_776 2_765
Se4B Sn1 Se4B 180.0(5) 11_566 2_765
Se4 Sn1 Se4B 98.1(5) . 12_656
Se4 Sn1 Se4B 81.9(5) 10_776 12_656
Se4 Sn1 Se4B 92.4(4) 11_566 12_656
Se4 Sn1 Se4B 87.6(4) 2_765 12_656
Se4 Sn1 Se4B 7.6(6) 12_656 12_656
Se4 Sn1 Se4B 172.4(6) 3_675 12_656
Se4B Sn1 Se4B 92.3(4) . 12_656
Se4B Sn1 Se4B 87.7(4) 10_776 12_656
Se4B Sn1 Se4B 87.7(4) 11_566 12_656
Se4B Sn1 Se4B 92.3(4) 2_765 12_656
Se4 Sn1 Se4B 81.9(5) . 3_675
Se4 Sn1 Se4B 98.1(5) 10_776 3_675
Se4 Sn1 Se4B 87.6(4) 11_566 3_675
Se4 Sn1 Se4B 92.4(4) 2_765 3_675
Se4 Sn1 Se4B 172.4(6) 12_656 3_675
Se4 Sn1 Se4B 7.6(6) 3_675 3_675
Se4B Sn1 Se4B 87.7(4) . 3_675
Se4B Sn1 Se4B 92.3(4) 10_776 3_675
Se4B Sn1 Se4B 92.3(4) 11_566 3_675
Se4B Sn1 Se4B 87.7(4) 2_765 3_675
Se4B Sn1 Se4B 180.0(5) 12_656 3_675
Se5B Cs2 Se5B 118.5(4) 1_455 3_675
Se5B Cs2 Se5B 118.5(4) 1_455 2_655
Se5B Cs2 Se5B 118.5(4) 3_675 2_655
Se5B Cs2 Se5A 57.4(10) 1_455 2_665
Se5B Cs2 Se5A 61.7(9) 3_675 2_665
Se5B Cs2 Se5A 166.2(10) 2_655 2_665
Se5B Cs2 Se5A 61.7(9) 1_455 3_565
Se5B Cs2 Se5A 166.2(10) 3_675 3_565
Se5B Cs2 Se5A 57.4(10) 2_655 3_565
Se5A Cs2 Se5A 118.74(15) 2_665 3_565
Se5B Cs2 Se5A 166.2(10) 1_455 .
Se5B Cs2 Se5A 57.4(10) 3_675 .
Se5B Cs2 Se5A 61.7(9) 2_655 .
Se5A Cs2 Se5A 118.74(15) 2_665 .
Se5A Cs2 Se5A 118.74(15) 3_565 .
Se5B Cs2 Se5 65.6(11) 1_455 17_455
Se5B Cs2 Se5 129.6(12) 3_675 17_455
Se5B Cs2 Se5 94.1(7) 2_655 17_455
Se5A Cs2 Se5 95.4(5) 2_665 17_455
Se5A Cs2 Se5 63.9(4) 3_565 17_455
Se5A Cs2 Se5 127.9(6) . 17_455
Se5B Cs2 Se5 94.1(6) 1_455 16_665
Se5B Cs2 Se5 65.6(11) 3_675 16_665
Se5B Cs2 Se5 129.6(12) 2_655 16_665
Se5A Cs2 Se5 63.9(4) 2_665 16_665
Se5A Cs2 Se5 127.9(6) 3_565 16_665
Se5A Cs2 Se5 95.4(5) . 16_665
Se5 Cs2 Se5 64.1(2) 17_455 16_665
Se5B Cs2 Se5 129.6(12) 1_455 18_545
Se5B Cs2 Se5 94.1(7) 3_675 18_545
Se5B Cs2 Se5 65.6(11) 2_655 18_545
Se5A Cs2 Se5 127.9(6) 2_665 18_545
Se5A Cs2 Se5 95.4(5) 3_565 18_545
Se5A Cs2 Se5 63.9(4) . 18_545
Se5 Cs2 Se5 64.1(2) 17_455 18_545
Se5 Cs2 Se5 64.1(2) 16_665 18_545
Se5B Cs2 P06 30.8(10) 1_455 2_665
Se5B Cs2 P06 89.0(7) 3_675 2_665
Se5B Cs2 P06 137.8(10) 2_655 2_665
Se5A Cs2 P06 32.2(5) 2_665 2_665
Se5A Cs2 P06 88.0(5) 3_565 2_665
Se5A Cs2 P06 139.2(5) . 2_665
Se5 Cs2 P06 90.6(3) 17_455 2_665
Se5 Cs2 P06 89.7(3) 16_665 2_665
Se5 Cs2 P06 149.12(17) 18_545 2_665
Se5B Cs2 P06 89.0(7) 1_455 3_565
Se5B Cs2 P06 137.8(10) 3_675 3_565
Se5B Cs2 P06 30.8(10) 2_655 3_565
Se5A Cs2 P06 139.2(5) 2_665 3_565
Se5A Cs2 P06 32.2(5) 3_565 3_565
Se5A Cs2 P06 88.0(5) . 3_565
Se5 Cs2 P06 89.7(3) 17_455 3_565
Se5 Cs2 P06 149.12(17) 16_665 3_565
Se5 Cs2 P06 90.5(3) 18_545 3_565
P06 Cs2 P06 107.53(13) 2_665 3_565
Se5B Cs2 P06 137.8(10) 1_455 .
Se5B Cs2 P06 30.8(10) 3_675 .
Se5B Cs2 P06 89.0(7) 2_655 .
Se5A Cs2 P06 88.0(5) 2_665 .
Se5A Cs2 P06 139.2(5) 3_565 .
Se5A Cs2 P06 32.2(5) . .
Se5 Cs2 P06 149.12(17) 17_455 .
Se5 Cs2 P06 90.6(3) 16_665 .
Se5 Cs2 P06 89.7(3) 18_545 .
P06 Cs2 P06 107.53(13) 2_665 .
P06 Cs2 P06 107.53(12) 3_565 .
Se4A Cs3 Se4A 119.975(13) 1_545 2_765
Se4A Cs3 Se4A 119.975(13) 1_545 3_565
Se4A Cs3 Se4A 119.975(14) 2_765 3_565
Se4A Cs3 Se4B 57.4(2) 1_545 3_665
Se4A Cs3 Se4B 62.6(2) 2_765 3_665
Se4A Cs3 Se4B 176.8(2) 3_565 3_665
Se4A Cs3 Se4B 62.6(2) 1_545 2_655
Se4A Cs3 Se4B 176.8(2) 2_765 2_655
Se4A Cs3 Se4B 57.4(2) 3_565 2_655
Se4B Cs3 Se4B 119.971(14) 3_665 2_655
Se4A Cs3 Se4B 176.8(2) 1_545 .
Se4A Cs3 Se4B 57.4(2) 2_765 .
Se4A Cs3 Se4B 62.6(2) 3_565 .
Se4B Cs3 Se4B 119.971(15) 3_665 .
Se4B Cs3 Se4B 119.971(16) 2_655 .
Se4A Cs3 P07 143.2(3) 1_545 .
Se4A Cs3 P07 36.2(3) 2_765 .
Se4A Cs3 P07 91.4(3) 3_565 .
Se4B Cs3 P07 91.7(3) 3_665 .
Se4B Cs3 P07 143.0(3) 2_655 .
Se4B Cs3 P07 36.0(3) . .
Se4A Cs3 P07 36.2(3) 1_545 3_665
Se4A Cs3 P07 91.4(3) 2_765 3_665
Se4A Cs3 P07 143.2(3) 3_565 3_665
Se4B Cs3 P07 36.0(3) 3_665 3_665
Se4B Cs3 P07 91.7(3) 2_655 3_665
Se4B Cs3 P07 143.0(3) . 3_665
P07 Cs3 P07 107.08(13) . 3_665
Se4A Cs3 P07 91.4(3) 1_545 2_655
Se4A Cs3 P07 143.2(3) 2_765 2_655
Se4A Cs3 P07 36.2(3) 3_565 2_655
Se4B Cs3 P07 143.0(3) 3_665 2_655
Se4B Cs3 P07 36.0(3) 2_655 2_655
Se4B Cs3 P07 91.7(3) . 2_655
P07 Cs3 P07 107.08(13) . 2_655
P07 Cs3 P07 107.08(13) 3_665 2_655
Se4A Cs3 Se5A 126.3(5) 1_545 .
Se4A Cs3 Se5A 60.7(7) 2_765 .
Se4A Cs3 Se5A 86.3(7) 3_565 .
Se4B Cs3 Se5A 96.8(7) 3_665 .
Se4B Cs3 Se5A 119.8(7) 2_655 .
Se4B Cs3 Se5A 54.8(5) . .
P07 Cs3 Se5A 30.0(5) . .
P07 Cs3 Se5A 94.2(5) 3_665 .
P07 Cs3 Se5A 85.9(8) 2_655 .
Se4A Cs3 Se5A 60.7(7) 1_545 3_665
Se4A Cs3 Se5A 86.3(8) 2_765 3_665
Se4A Cs3 Se5A 126.3(5) 3_565 3_665
Se4B Cs3 Se5A 54.8(4) 3_665 3_665
Se4B Cs3 Se5A 96.8(8) 2_655 3_665
Se4B Cs3 Se5A 119.8(7) . 3_665
P07 Cs3 Se5A 85.9(8) . 3_665
P07 Cs3 Se5A 30.0(5) 3_665 3_665
P07 Cs3 Se5A 94.2(5) 2_655 3_665
Se5A Cs3 Se5A 66.0(7) . 3_665
Se4A Cs3 Se5A 86.3(7) 1_545 2_655
Se4A Cs3 Se5A 126.3(5) 2_765 2_655
Se4A Cs3 Se5A 60.7(7) 3_565 2_655
Se4B Cs3 Se5A 119.8(7) 3_665 2_655
Se4B Cs3 Se5A 54.8(5) 2_655 2_655
Se4B Cs3 Se5A 96.8(7) . 2_655
P07 Cs3 Se5A 94.2(5) . 2_655
P07 Cs3 Se5A 85.9(8) 3_665 2_655
P07 Cs3 Se5A 30.0(5) 2_655 2_655
Se5A Cs3 Se5A 66.0(7) . 2_655
Se5A Cs3 Se5A 66.0(7) 3_665 2_655
P06 Se4 P07 30.9(3) . .
P06 Se4 P07 30.7(3) . 3_675
P07 Se4 P07 51.5(4) . 3_675
P06 Se4 Sn1 98.9(3) . .
P07 Se4 Sn1 82.2(5) . .
P07 Se4 Sn1 82.2(4) 3_675 .
P06 Se4 Cs3 89.8(10) . .
P07 Se4 Cs3 64.9(9) . .
P07 Se4 Cs3 116.3(9) 3_675 .
Sn1 Se4 Cs3 93.1(9) . .
P06 Se4 Cs3 89.5(10) . 1_565
P07 Se4 Cs3 116.2(9) . 1_565
P07 Se4 Cs3 64.8(9) 3_675 1_565
Sn1 Se4 Cs3 93.0(8) . 1_565
Cs3 Se4 Cs3 173.9(3) . 1_565
P06 Se4 Cs3 172.1(4) . 10_666
P07 Se4 Cs3 152.8(13) . 10_666
P07 Se4 Cs3 152.5(13) 3_675 10_666
Sn1 Se4 Cs3 89.03(17) . 10_666
Cs3 Se4 Cs3 90.0(5) . 10_666
Cs3 Se4 Cs3 89.9(5) 1_565 10_666
P06 Se4 Cs2 64.0(3) . .
P07 Se4 Cs2 82.4(3) . .
P07 Se4 Cs2 82.4(4) 3_675 .
Sn1 Se4 Cs2 162.9(2) . .
Cs3 Se4 Cs2 87.2(5) . .
Cs3 Se4 Cs2 87.1(5) 1_565 .
Cs3 Se4 Cs2 108.06(18) 10_666 .
Se4B Se4A P07 106(2) . 3_675
Se4B Se4A P06 80.4(18) . .
P07 Se4A P06 31.3(3) 3_675 .
Se4B Se4A P07 56.1(18) . .
P07 Se4A P07 49.8(5) 3_675 .
P06 Se4A P07 28.9(3) . .
Se4B Se4A Sn1 81(3) . .
P07 Se4A Sn1 80.9(5) 3_675 .
P06 Se4A Sn1 94.4(6) . .
P07 Se4A Sn1 75.8(5) . .
Se4B Se4A Cs3 179(2) . 1_565
P07 Se4A Cs3 73.5(5) 3_675 1_565
P06 Se4A Cs3 99.0(6) . 1_565
P07 Se4A Cs3 123.3(5) . 1_565
Sn1 Se4A Cs3 99.1(4) . 1_565
Se4B Se4A Cs2 86(2) . .
P07 Se4A Cs2 85.9(5) 3_675 .
P06 Se4A Cs2 65.9(4) . .
P07 Se4A Cs2 82.2(4) . .
Sn1 Se4A Cs2 158.0(5) . .
Cs3 Se4A Cs2 93.8(5) 1_565 .
Se4B Se4A Cs3 85.4(18) . 10_666
P07 Se4A Cs3 161.8(6) 3_675 10_666
P06 Se4A Cs3 165.3(7) . 10_666
P07 Se4A Cs3 139.5(7) . 10_666
Sn1 Se4A Cs3 86.9(3) . 10_666
Cs3 Se4A Cs3 95.3(3) 1_565 10_666
Cs2 Se4A Cs3 109.6(3) . 10_666
Se4B Se4A Cs3 3(2) . .
P07 Se4A Cs3 107.0(6) 3_675 .
P06 Se4A Cs3 80.7(5) . .
P07 Se4A Cs3 57.2(4) . .
Sn1 Se4A Cs3 83.5(5) . .
Cs3 Se4A Cs3 177.3(5) 1_565 .
Cs2 Se4A Cs3 83.6(3) . .
Cs3 Se4A Cs3 84.9(3) 10_666 .
Se4A Se4B P07 108(2) . .
Se4A Se4B P06 81.1(18) . .
P07 Se4B P06 31.5(3) . .
Se4A Se4B P07 57.7(18) . 3_675
P07 Se4B P07 50.0(5) . 3_675
P06 Se4B P07 28.9(3) . 3_675
Se4A Se4B Sn1 84(3) . .
P07 Se4B Sn1 81.5(5) . .
P06 Se4B Sn1 95.0(6) . .
P07 Se4B Sn1 76.3(5) 3_675 .
Se4A Se4B Cs3 177(3) . .
P07 Se4B Cs3 73.6(5) . .
P06 Se4B Cs3 99.2(6) . .
P07 Se4B Cs3 123.5(5) 3_675 .
Sn1 Se4B Cs3 99.4(4) . .
Se4A Se4B Cs2 84(2) . .
P07 Se4B Cs2 85.6(5) . .
P06 Se4B Cs2 65.6(4) . .
P07 Se4B Cs2 82.0(4) 3_675 .
Sn1 Se4B Cs2 158.3(5) . .
Cs3 Se4B Cs2 93.5(4) . .
Se4A Se4B Cs3 84.3(18) . 10_666
P07 Se4B Cs3 162.2(5) . 10_666
P06 Se4B Cs3 165.0(6) . 10_666
P07 Se4B Cs3 139.6(7) 3_675 10_666
Sn1 Se4B Cs3 87.0(4) . 10_666
Cs3 Se4B Cs3 95.1(3) . 10_666
Cs2 Se4B Cs3 109.2(3) . 10_666
Se4A Se4B Cs3 0.5(18) . 1_565
P07 Se4B Cs3 107.2(6) . 1_565
P06 Se4B Cs3 80.6(5) . 1_565
P07 Se4B Cs3 57.3(4) 3_675 1_565
Sn1 Se4B Cs3 83.7(5) . 1_565
Cs3 Se4B Cs3 176.8(5) . 1_565
Cs2 Se4B Cs3 83.5(2) . 1_565
Cs3 Se4B Cs3 84.8(3) 10_666 1_565
P07 Se5 P06 32.5(4) . 2_765
P07 Se5 P06 32.2(3) . .
P06 Se5 P06 44.6(4) 2_765 .
P07 Se5 Cs3 71.0(3) . .
P06 Se5 Cs3 94.9(3) 2_765 .
P06 Se5 Cs3 94.5(3) . .
P07 Se5 Cs2 107.7(3) . 16_665
P06 Se5 Cs2 84.3(3) 2_765 16_665
P06 Se5 Cs2 83.9(3) . 16_665
Cs3 Se5 Cs2 178.3(4) . 16_665
P07 Se5 Cs2 93.9(7) . 1_655
P06 Se5 Cs2 70.1(5) 2_765 1_655
P06 Se5 Cs2 114.6(6) . 1_655
Cs3 Se5 Cs2 94.2(3) . 1_655
Cs2 Se5 Cs2 86.9(3) 16_665 1_655
P07 Se5 Cs2 91.8(7) . .
P06 Se5 Cs2 112.9(6) 2_765 .
P06 Se5 Cs2 68.3(5) . .
Cs3 Se5 Cs2 93.0(4) . .
Cs2 Se5 Cs2 85.9(3) 16_665 .
Cs2 Se5 Cs2 171.91(19) 1_655 .
Se5B Se5A P07 75(3) . .
Se5B Se5A P06 100(4) . .
P07 Se5A P06 36.1(6) . .
Se5B Se5A P06 53(3) . 2_765
P07 Se5A P06 31.9(8) . 2_765
P06 Se5A P06 46.4(9) . 2_765
Se5B Se5A Cs2 173(4) . .
P07 Se5A Cs2 105.7(13) . .
P06 Se5A Cs2 78.4(12) . .
P06 Se5A Cs2 124.6(10) 2_765 .
Se5B Se5A Cs3 87(4) . .
P07 Se5A Cs3 73.0(8) . .
P06 Se5A Cs3 100.5(9) . .
P06 Se5A Cs3 95.3(11) 2_765 .
Cs2 Se5A Cs3 99.9(9) . .
Se5B Se5A Cs2 84(4) . 16_665
P07 Se5A Cs2 108.2(12) . 16_665
P06 Se5A Cs2 85.1(9) . 16_665
P06 Se5A Cs2 82.0(8) 2_765 16_665
Cs2 Se5A Cs2 89.9(8) . 16_665
Cs3 Se5A Cs2 169.5(12) . 16_665
Se5B Se5A Cs2 9(4) . 1_655
P07 Se5A Cs2 84.7(16) . 1_655
P06 Se5A Cs2 108.2(16) . 1_655
P06 Se5A Cs2 61.9(10) 2_765 1_655
Cs2 Se5A Cs2 168.0(8) . 1_655
Cs3 Se5A Cs2 88.9(8) . 1_655
Cs2 Se5A Cs2 80.8(6) 16_665 1_655
Se5A Se5B P07 80(3) . .
Se5A Se5B P06 107(4) . 2_765
P07 Se5B P06 37.5(12) . 2_765
Se5A Se5B P06 60(3) . .
P07 Se5B P06 31.7(10) . .
P06 Se5B P06 47.0(12) 2_765 .
Se5A Se5B Cs2 169(5) . 1_655
P07 Se5B Cs2 111(4) . 1_655
P06 Se5B Cs2 83(3) 2_765 1_655
P06 Se5B Cs2 130(3) . 1_655
Se5A Se5B Cs3 81(4) . .
P07 Se5B Cs3 72.1(13) . .
P06 Se5B Cs3 101.4(17) 2_765 .
P06 Se5B Cs3 94.2(15) . .
Cs2 Se5B Cs3 101.5(16) 1_655 .
Se5A Se5B Cs2 84(4) . 16_665
P07 Se5B Cs2 109.2(17) . 16_665
P06 Se5B Cs2 86.7(13) 2_765 16_665
P06 Se5B Cs2 82.0(12) . 16_665
Cs2 Se5B Cs2 91.9(13) 1_655 16_665
Cs3 Se5B Cs2 165(3) . 16_665
P07 P06 P07 110.9(10) 3_675 .
P07 P06 P06 45.0(7) 3_675 3_675
P07 P06 P06 96.5(6) . 3_675
P07 P06 P06 96.7(6) 3_675 2_765
P07 P06 P06 44.8(7) . 2_765
P06 P06 P06 59.999(9) 3_675 2_765
P07 P06 Se5B 67(2) 3_675 3_675
P07 P06 Se5B 174(3) . 3_675
P06 P06 Se5B 78(3) 3_675 3_675
P06 P06 Se5B 129(2) 2_765 3_675
P07 P06 Se5A 171.1(15) 3_675 .
P07 P06 Se5A 64.5(13) . .
P06 P06 Se5A 126.6(12) 3_675 .
P06 P06 Se5A 74.6(14) 2_765 .
Se5B P06 Se5A 117(2) 3_675 .
P07 P06 P07 63.7(5) 3_675 2_765
P07 P06 P07 63.7(5) . 2_765
P06 P06 P07 32.9(3) 3_675 2_765
P06 P06 P07 33.0(3) 2_765 2_765
Se5B P06 P07 111(3) 3_675 2_765
Se5A P06 P07 107.6(14) . 2_765
P07 P06 Se5 62.0(6) 3_675 3_675
P07 P06 Se5 164.6(9) . 3_675
P06 P06 Se5 68.7(8) 3_675 3_675
P06 P06 Se5 120.5(6) 2_765 3_675
Se5B P06 Se5 10(2) 3_675 3_675
Se5A P06 Se5 120.4(9) . 3_675
P07 P06 Se5 101.5(7) 2_765 3_675
P07 P06 Se4 76.5(9) 3_675 .
P07 P06 Se4 76.2(10) . .
P06 P06 Se4 114.4(6) 3_675 .
P06 P06 Se4 114.2(7) 2_765 .
Se5B P06 Se4 108.2(18) 3_675 .
Se5A P06 Se4 108.6(12) . .
P07 P06 Se4 104.0(4) 2_765 .
Se5 P06 Se4 113.0(10) 3_675 .
P07 P06 Se5 162.9(9) 3_675 .
P07 P06 Se5 60.7(6) . .
P06 P06 Se5 118.7(7) 3_675 .
P06 P06 Se5 66.7(7) 2_765 .
Se5B P06 Se5 119.5(14) 3_675 .
Se5A P06 Se5 8.2(12) . .
P07 P06 Se5 99.6(7) 2_765 .
Se5 P06 Se5 121.8(4) 3_675 .
Se4 P06 Se5 113.2(10) . .
P07 P06 Se4B 85.5(8) 3_675 .
P07 P06 Se4B 69.9(6) . .
P06 P06 Se4B 121.3(6) 3_675 .
P06 P06 Se4B 110.9(5) 2_765 .
Se5B P06 Se4B 114.9(17) 3_675 .
Se5A P06 Se4B 99.3(10) . .
P07 P06 Se4B 106.2(5) 2_765 .
Se5 P06 Se4B 120.7(6) 3_675 .
Se4 P06 Se4B 9.4(5) . .
Se5 P06 Se4B 103.7(6) . .
P07 P06 Se5A 54.5(8) 3_675 3_675
P07 P06 Se5A 155.4(12) . 3_675
P06 P06 Se5A 59.0(10) 3_675 3_675
P06 P06 Se5A 113.0(10) 2_765 3_675
Se5B P06 Se5A 19(2) 3_675 3_675
Se5A P06 Se5A 126.7(13) . 3_675
P07 P06 Se5A 91.8(10) 2_765 3_675
Se5 P06 Se5A 9.9(5) 3_675 3_675
Se4 P06 Se5A 114.0(12) . 3_675
Se5 P06 Se5A 126.7(6) . 3_675
Se4B P06 Se5A 122.6(9) . 3_675
P06 P07 P06 90.1(10) 2_765 .
P06 P07 Se5B 75(2) 2_765 .
P06 P07 Se5B 96(2) . .
P06 P07 Se5A 93.6(13) 2_765 .
P06 P07 Se5A 79.5(12) . .
Se5B P07 Se5A 25(3) . .
P06 P07 Se5 85.4(7) 2_765 .
P06 P07 Se5 87.1(7) . .
Se5B P07 Se5 13(2) . .
Se5A P07 Se5 11.1(10) . .
P06 P07 P07 34.6(6) 2_765 2_765
P06 P07 P07 83.3(6) . 2_765
Se5B P07 P07 110(2) . 2_765
Se5A P07 P07 125.1(11) . 2_765
Se5 P07 P07 118.8(5) . 2_765
P06 P07 P07 83.4(5) 2_765 3_675
P06 P07 P07 34.5(6) . 3_675
Se5B P07 P07 126.0(16) . 3_675
Se5A P07 P07 113.6(11) . 3_675
Se5 P07 P07 120.0(5) . 3_675
P07 P07 P07 60.001(4) 2_765 3_675
P06 P07 Se4B 152.7(9) 2_765 .
P06 P07 Se4B 78.6(7) . .
Se5B P07 Se4B 130(3) . .
Se5A P07 Se4B 108.4(14) . .
Se5 P07 Se4B 118.3(9) . .
P07 P07 Se4B 118.5(7) 2_765 .
P07 P07 Se4B 73.2(7) 3_675 .
P06 P07 Se4A 78.4(7) 2_765 2_765
P06 P07 Se4A 152.8(9) . 2_765
Se5B P07 Se4A 105(3) . 2_765
Se5A P07 Se4A 125.3(13) . 2_765
Se5 P07 Se4A 116.1(8) . 2_765
P07 P07 Se4A 73.2(7) 2_765 2_765
P07 P07 Se4A 118.8(7) 3_675 2_765
Se4B P07 Se4A 100.5(5) . 2_765
P06 P07 P06 50.4(5) 2_765 3_675
P06 P07 P06 50.4(5) . 3_675
Se5B P07 P06 108.5(14) . 3_675
Se5A P07 P06 110.2(9) . 3_675
Se5 P07 P06 110.2(4) . 3_675
P07 P07 P06 32.9(3) 2_765 3_675
P07 P07 P06 33.0(3) 3_675 3_675
Se4B P07 P06 105.2(7) . 3_675
Se4A P07 P06 105.2(7) 2_765 3_675
P06 P07 Se4 143.9(10) 2_765 .
P06 P07 Se4 72.9(9) . .
Se5B P07 Se4 137(3) . .
Se5A P07 Se4 113.5(14) . .
Se5 P07 Se4 124.0(8) . .
P07 P07 Se4 110.2(7) 2_765 .
P07 P07 Se4 64.4(9) 3_675 .
Se4B P07 Se4 9.1(4) . .
Se4A P07 Se4 102.2(7) 2_765 .
P06 P07 Se4 96.2(9) 3_675 .
P06 P07 Se4 72.8(9) 2_765 2_765
P06 P07 Se4 143.5(11) . 2_765
Se5B P07 Se4 110(3) . 2_765
Se5A P07 Se4 132.2(14) . 2_765
Se5 P07 Se4 122.1(8) . 2_765
P07 P07 Se4 64.2(9) 2_765 2_765
P07 P07 Se4 110.0(8) 3_675 2_765
Se4B P07 Se4 101.9(6) . 2_765
Se4A P07 Se4 9.5(4) 2_765 2_765
P06 P07 Se4 95.9(10) 3_675 2_765
Se4 P07 Se4 102.1(5) . 2_765
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sn1 Se4 2.622(9) .
Sn1 Se4 2.622(9) 10_776
Sn1 Se4 2.622(8) 11_566
Sn1 Se4 2.622(8) 2_765
Sn1 Se4 2.622(8) 12_656
Sn1 Se4 2.622(8) 3_675
Sn1 Se4B 2.745(18) .
Sn1 Se4B 2.745(18) 10_776
Sn1 Se4B 2.745(18) 11_566
Sn1 Se4B 2.745(18) 2_765
Sn1 Se4B 2.745(18) 12_656
Sn1 Se4B 2.745(18) 3_675
Cs2 Se5B 3.47(9) 1_455
Cs2 Se5B 3.47(9) 3_675
Cs2 Se5B 3.47(9) 2_655
Cs2 Se5A 3.60(5) 2_665
Cs2 Se5A 3.60(5) 3_565
Cs2 Se5A 3.60(5) .
Cs2 Se5 3.759(5) 17_455
Cs2 Se5 3.759(5) 16_665
Cs2 Se5 3.759(5) 18_545
Cs2 P06 3.766(8) 2_665
Cs2 P06 3.766(8) 3_565
Cs2 P06 3.766(8) .
Cs3 Se4A 3.54(2) 1_545
Cs3 Se4A 3.54(2) 2_765
Cs3 Se4A 3.54(2) 3_565
Cs3 Se4B 3.538(18) 3_665
Cs3 Se4B 3.538(18) 2_655
Cs3 Se4B 3.538(18) .
Cs3 P07 3.601(9) .
Cs3 P07 3.601(9) 3_665
Cs3 P07 3.601(9) 2_655
Cs3 Se5A 3.67(3) .
Cs3 Se5A 3.67(3) 3_665
Cs3 Se5A 3.67(3) 2_655
Se4 P06 2.283(10) .
Se4 P07 2.321(19) .
Se4 P07 2.325(19) 3_675
Se4 Cs3 3.91(4) 1_565
Se4 Cs3 4.090(6) 10_666
Se4A Se4B 0.738(16) .
Se4A P07 2.216(16) 3_675
Se4A P06 2.306(15) .
Se4A P07 2.529(18) .
Se4A Cs3 3.54(2) 1_565
Se4A Cs3 4.102(13) 10_666
Se4B P07 2.205(16) .
Se4B P06 2.301(15) .
Se4B P07 2.520(18) 3_675
Se4B Cs3 4.109(13) 10_666
Se4B Cs3 4.274(17) 1_565
Se5 P07 2.008(11) .
Se5 P06 2.265(15) 2_765
Se5 P06 2.298(14) .
Se5 Cs2 3.759(5) 16_665
Se5 Cs2 3.88(2) 1_655
Se5A Se5B 0.79(9) .
Se5A P07 1.88(3) .
Se5A P06 2.05(3) .
Se5A P06 2.31(4) 2_765
Se5A Cs2 3.83(3) 16_665
Se5A Cs2 4.25(4) 1_655
Se5B P07 1.85(5) .
Se5B P06 1.94(6) 2_765
Se5B P06 2.32(6) .
Se5B Cs2 3.47(9) 1_655
Se5B Cs2 3.83(4) 16_665
P06 P07 1.222(12) 3_675
P06 P07 1.227(12) .
P06 P06 1.734(15) 3_675
P06 P06 1.734(15) 2_765
P06 Se5B 1.94(6) 3_675
P06 P07 2.235(12) 2_765
P06 Se5 2.265(14) 3_675
P06 Se5A 2.31(4) 3_675
P07 P06 1.222(12) 2_765
P07 P07 2.016(15) 2_765
P07 P07 2.016(15) 3_675
P07 Se4A 2.216(15) 2_765
P07 P06 2.235(12) 3_675
P07 Se4 2.325(18) 2_765
